IMMEDIAL  COLOURS 

ON 

LOOSE  COTTON 


CASSELLA  COLOR  COMPANY 

182  and  184  Front  Street, 

NEW  YORK. 

Boston;  39  Oliver  Street, 

Philadelphia:  126  and  128  South  Front  Street. 
Providence:  64  Exchangee  Place. 

Atlanta:  47  North  Pryor  Street. 

Montreal. Canada, 59. William  Street. 


No.  5598 


LEOPOLD  CASSELLA  & Co.,  G.  m.  b.  H.,  FRANKFORT 


Works  at^Mainkur  near  Frankfort 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


CASSELLA  COEOR;  COMPANY 

182  AND  184  FRONT  STREET 

NEW  YORK 


BOSTON:  39  Oliver  street 
PHILADELPHIA:  126  and  128  south  front  street 
PROVIDENCE:  64  exchange  place 
ATLANTA:  north  pryor  street 

MONTREAL:  Canada,  59  william  street. 


No  3398. 


f 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON. 


Immedial  Colours  are  dyed  on  loose  cotton  either  in  vats  or  kettles 
or  in  mechanical  apparatus.  The  parts  of  the  vessels  or  fittings  which 
come  into  contact  with  the  liquor  must  not  be  made  of  copper  or  brass. 

For  heating  the  liquor,  it  is  best  to  use  indirect  steam,  the  heating 
pipes  being  made  either  of  iron  or  lead. 

The  dyeing  is  done  with  the  addition  of  sodium  sulphide  and  soda, 
besides  which  common  salt  or  Glauber’s  salt  are  added  for  medium  and 
deep  shades. 


Additions  to  the  Bath: 


The  following  are  the  ingredients  used  as  a rule : 


For: 


Immedial  Black  “extra”  and 

plain  brands 
Immedial  Black  “concentrated” 
Immedial  Carbon 
Indo  Carbon 
Immedial  Blue 

Immedial  Blue  “extra  cone.” 
Immedial  Direct  Blue 
Immedial  Direct  Blue 

“extra  cone.” 
Immedial  Indone  Violet 
Immedial  Indone 
Immedial  Indogene 
Immedial  Dark  Blue 
Immedial  New  Blue 
Immedial  Brilliant  Green 
Immedial  Green 
Immedial  Deep  Green 
Immedial  Dark  Green 
Immedial  Olive 


Sodium 
Sulphide  cryst. 
per  1 part 
dyestuff. 

I Parts : 


72—^4 


Soda  Ash 


1 

172-2 

172—2 

3/4-1 

172-2 

1 


4 8 oz 
per  10  gallons 
liquor 

for  the  first 
bath,  and 
Vi— V2°/o  of  the 
weight  of  the 
goods  for 
subsequent 
dyeing. 


172—2 


1 


In  order  to 
obtain  brighter 
shades  when 
developing 
Immedial  Blue 
and  Immedial 
New  Blue  by 
steaming  or 
storing,  the 
soda  may  be 
replaced  by 
about  one-half 
its  weight  of 
caustic  soda  lye 
770  Tw. 


Common  Salt 
or  desiccated 
Glauber’s  Salt 


Depending  on 
the  depth  of  the 
shade,  0—2  lbs, 
for  Black  up  to 
3 lbs  per 
10  gallons  for 
' the  first  bath, 
and  0— 5®/o 
of  the  weight 
of  the  goods 
for  subsequent 
lots. 


• Instead  of  the  quantities  of  sodium  sulphide  crystals  indicated,  half  the  amount 
of  sodium  sulphide  cone,  may  be  used. 


1 


For: 

Sodium  ' 

Sulphide  cry  St.* 
per  1 part 
dyestuff. 
Parts: 

Soda  ash 

Common  salt 
or  desiccated 
Glauber’s  salt 

Immedial  Green  Yellow 
Immedial  Yellow 
Immedial  Orange 
Immedial  Cutch 
Immedial  Brown 
Immedial  Yellow  Brown 
Immedial  Deep  Brown 
Immedial  Dark  Brown 
Immedial  Bronze 
Immedial  Prune 
Immedial  Red  Brown 
Immedial  Bordeaux 
Immedial  Maroon 
Immedial  Violet 
Immedial  Purple 

1 part 

4—8  oz 

per  10  gallons 
liquor 

for  the  first 
bath  and 

V»  — '/2®/0 

of  ihe  weight 
of  the  goods 
for  subsequent 
lots. 

Depending  on 
the  depth  of  the 
shade  to  be 
dyed,  0—2  lbs, 
for  Black  up  to 
3 lbs  per 
10  gallons  for 
the  first  bath, 
and  0 — 5®/o 
of  the  weight 
of  the  goods 
for  subsequent 
lots. 

The  quantities  of  dyestuff  to  be  added  depend  on  the  volume  of 
liquor;  the  more  dilute  the  liquor,  the  more  dyestuff  will  be  required  for 
the  first  bath.  With  a volume  of  liquor  of  about  15  times  the  weight  of 
the  goods  to  be  dyed,  about  two-thirds  to  three-quarters  the  weights 
used  originally  should  be  added  for  subsequent  lots. 

Dyeing.  As  a rule,  the  dry,  previously  opened  cotton  is  entered 
into  the  boiling  bath,  and  then  dyed  for  *,2  to  1 hour  near  boiling  temperature, 
or,  the  dyeing  is  done  for  10  to  20  minutes  at  the  boil  and  then  continued 
with  the  steam  shut  off. 

In  the  case  of  colours  which  are  dyed  at  a lower  temperature  in 
order  to  produce  brighter  shades,  the  cotton  should  be  previously  boiled 
or  wetted  out. 

Rinsing.  When  working  in  open  kettles  or  vats,  the  cotton,  after 
the  dyeing,  is  thrown  on  to  wooden  lattice  frames  or  into  baskets  to 
allow  the  adhering  liquor  to  drain  into  the  dyebath,  and  is  then  rinsed. 

An  alternative  plan  is  to  whizz  first,  the  liquor  coming  off  being 
returned  to  the  bath,  and  to  then  rinse. 

When  working  in  machines,  the  liquor  is  pumped  into  the  reservoir 
after  the  dyeing,  whereupon  the  goods  are  whizzed  and  then  usually 
rinsed.  If  no  hydroextractor  be  available,  the  goods  are  straightaway 
rinsed  after  the  liquor  has  been  drawn  off  or  allowed  to  run  off. 

In  the  case  of  Blacks  (Indo  Carbon  excepted),  some  acetate  or  formate 
of  soda  or  carbonate  of  soda  are  added  to  the  final  rinsing  bath  if  the 
goods  are  not  to  be  given  an  alkaline  brightening  or  softening. 

* Instead  of  the  quantities  of  sodium  sulphide  crystals  indicated,  half  the  amount 
of  sodium  sulphide  cone,  may  be  used. 


2 


Dyeings  of  Immedial  Blue  and  Immedial  New  Blue  are  frequently 
not  rinsed  immediately  after  the  dyeing,  but  instead  are  hydroextracted, 
and  then  developed  by  steaming  or  smothering,  being  only  then  rinsed. 


Full  particulars  with  regard  to  the  charging  of  the  dyebaths  and 
the  additions  for  subsequent  lots,  as  well  as  other  details  regarding  the 
dyeing,  are  to  be  found  in  our  “Manual  of  Dyeing”,  Vol.  I,  No  2938,  2"'’- 
edition,  pages  22  et  seq.  and  pages  60-62,  for  machine-dyeing  in  the 
same  Manual  of  Dyeing,  section  3 on  “Machine  Dyeing”. 


Aftertreatments.  Dyeings  of  Immedial  Colours  are  frequently 
aftertreated  after  the  dyeing,  for  which  purpose  the  following  methods 
come  into  consideration: 

I.  Aftertreatment  with  Metallic  Salts. 

a)  Aftertreatment  with  bichrome 

b)  Aftertreatment  with  bichrome  and  sulphate  of  copper 

c)  Aftertreatment  with  bichrome  and  bisulphite 

d)  Aftertreatment  with  bichrome  and  nickel  sulphate. 

II.  Aftertreatment  with  Acetate  and  Formate  of  Soda. 

III.  Aftertreatment  with  Immedial  Developer. 

IV.  Developing  of  Immedial  Blue  and  Immedial  New  Blue  by  Steaming 

or  Smothering. 

For  fuller  particulars  see  our  “Manual  of  Dyeing”,  Vol.  I.,  No  2938, 
2"'*-  edition,  pages  35 — 39. 


The  quantities  of  dyestuff  indicated  in  the  card  are  those  actually 
absorbed  and  required  when  dyeing  subsequent  lots  on  the  standing  bath. 
The  standing  baths  have  to  be  correspondingly  stronger,  varying  with 
the  volume  of  the  liquor  used,  in  accordance  with  our  directions. 


Without  guarantee. 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


1. 

3 % Immedial  Yellow  GG  pat. 

2. 

6 % Immedial  Yellow  GG  pat. 

3. 

3 % Immedial  Yellow  D pat. 

4. 

6 % Immedial  Y-ellow  D pat. 

5. 

3 % Immedial  Orange  C pat. 

6. 

6 % Immedial  Orange  C pat. 

7. 

3,5%  Immedial  Cutch  0 pat. 

8. 

7 % Immedial  Cutch  0 pat. 

9. 

4 % Immedial  Cutch  G pat. 

10. 

8 % Immedial  Cutch  G pat. 

11. 

4 % Immedial  Cutch  R pot. 

12. 

8 % Immedial  Cutch  R pat. 

13. 

4 % Immedial  Cutch  OG  pat. 

14. 

8 % Immedial  Cutch  OG  pat. 

15. 

4 % Immedial  Cutch  OR  pat. 

16. 

8 % Immedial  Cutch  OR  pat. 

17. 

4 % Immedial  Cutch  BGG  pat. 

18. 

8 % Immedial  Cutch  BGG  pat. 


19, 

% Immedial  Cutch  BG  pat. 

20. 

% Immedial  Cutch  BG  pat. 

21. 

% Immedial  Dark  Brown  D cone.  pat. 
22. 

% Immedial  Dark  Brown  D cone.  pat. 

23. 

% Immedial  Dark  Brown  DN  cone.  pat. 

24. 

% Immedial  Dark  Brown  DN  cone.  pat. 

25. 

% Immedial  Brown  BR. 

26. 

% Immedial  Brown  BR. 

27. 

% Immedial  Brown  BRS. 

28. 

% Immedial  Brown  BRS. 

29. 

% Immedial  Brown  RR  pat. 

30. 

% Immedial  Brown  RR  pat. 

31. 

% Immedial  Brown  W cone.  pat. 

32. 

% Immedial  Brown  W cone.  pat. 

33. 

% Immedial  Red  Brown  3R  pat. 

34. 

% Immedial  Red  Brown  3R  pat. 

35. 

% Immedial  Prune  S pat. 

36. 

% Immedial  Prune  8 pat. 


4 

8 

4 

8 

4 

8 

4 

8 

4 

8 

4 

8 

4 

8 

4 

8 

4 

8 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


I 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


4 % 

Immedial 

37. 

Green  Blue  CV  pat. 

4 ^ 

/g  Immedial 

8 % 

Immedial 

38. 

Green  Blue  CV  pat. 

8 ^ 

fg  Immedial 

3.5% 

Immedial 

39. 

Green  BBX  cone.  pat. 

4 0 

/g  Immedial 

7 % 

Immedial 

40. 

Green  BBX  cone.  pat. 

8 « 

/g  Immedial 

3.5% 

Immedial 

41. 

Green  BB  extra  pat. 

4 0 

!g  Immedial 

7 % 

Immedial 

42. 

Green  BB  extra  pat. 

8 « 

!g  Immedial 

3.5% 

Immedial 

43. 

Deep  Green  G pat. 

4 

!g  Immedial 

7 % 

Immedial 

44. 

Deep  Green  G pat. 

8 

!g  Immedial 

3.5% 

Immedial 

45. 

Green  GG  extra  pat. 

4 

» 

!g  Immedial 

7 % 

Immedial 

46. 

Green  GG  extra  pat. 

8 

^ Immedial 

3.5% 

Immedial 

47. 

Green  GGX  cone.  pat. 

3 

Ig  Immedial 

7 % 

Immedial 

48. 

Green  GGX  cone.  pat. 

6 c 

!g  Immedial 

3.5% 

Immedial 

49. 

Brilliant  Green  G extra  pat. 

4 

!g  Immedial 

7 % 

Immedial 

50. 

Brilliant  Green  G extra  pat. 

8 

^ Immedial 

4 % 

Immedial 

51. 

Dark  Green  B. 

3 

Ig  Immedial 

8 % 

Immedial 

52. 

Dark  Green  B. 

6 

^ Immedial 

4 % 

Immedial 

53. 

Olive  GG  pat. 

4 « 

Ig  Immedial 

8 % 

Immedial 

54. 

Olive  GG  pat. 

8 « 

Ig  Immedial 

55. 

Olive  B pat. 

56. 

Olive  B pat. 

57. 

Olive  3G. 

58. 

Olive  3G. 

59. 

Green  Yellow  G pat. 

60. 

Green  Yellow  G pat. 

61. 

Yellow  Olive  5G  pat. 
62. 

Yellow  Olive  5G  pat. 

63. 

Yellow  Olive  G pat. 

64. 

Yellow  Olive  G pat. 

65. 

Khaki  G pat. 

66. 

Khaki  G pat. 

67. 

Yellow  Brown  EN  pat. 

68. 

Yellow  Brown  EN  pat. 

69. 

Khaki  D pat. 

70. 

Khaki  D pat. 

71. 

Dark  Brown  A pat. 

72. 

Dark  Brown  A pat. 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


u 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


73. 


6 % Immedial  Violet  CB  pat. 


74. 


12  % Immedial  Violet  CB  pat. 


75. 


6 % Immedial  Violet  C pat. 


76. 


12  % Immedial  Violet  C pat. 


77. 


6 % Immedial  Violet  CB  pat. 


78. 


12  % Immedial  Violet  CB  pat. 


79. 


6 % Immedial  Purple  C pat. 


80. 


12  % Immedial  Purple  C pat. 


81. 


3 % Immedial  Maroon  B cone.  pat. 


82. 


6  % Immedial  Maroon  B cone.  pat. 


83. 


3.5%  Immedial  Bordeaux  GF  cone.  pat. 


84. 


7  % Immedial  Bordeaux  GF  cone.  pat. 


85. 


4 % Immedial  Indogene  GCL  cone.  pat. 


86. 


8  % Immedial  Indogene  GCL  cone.  pat. 


87. 


3.5%  Immedial  Indogene  BCL  cone.  pat. 


88. 


7 % Immedial  Indogene  BCL  cone.  pat. 


89. 


3.5%  Immedial  Indogene  BCL  cone.  pat. 


90. 


7 % Immedial  Indogene  BCL  cone.  pat. 


91. 


3.5%  Immedial  Indogene  BBCL  cone.  pat. 


92. 


7 % Immedial  Indogene  BBCL  cone.  pat. 


93. 


3.5%  Immedial  Indogene  B cone.  pat. 


94. 


% Immedial  Indogene  B cone.  pat. 


95. 


3.5%  Immedial  Indone  JBF  cone.  pat. 


96. 


7 % Immedial  Indone  JBF  cone.  pat. 


97. 


3.5%  Immedial  Indone  BBF  cone.  pat. 


98. 


7 % Immedial  Indone  BBF  cone.  pat. 


99. 


3.5%  Immedial  Indone  JBN  cone.  pat. 


100. 


% Immedial  Indone  JBN  cone.  pat. 


101. 


3.5%  Immedial  Indone  B cone.  pat. 


102. 


7 % Immedial  Indone  B cone.  pat. 


103. 


3.5%  Immedial  Indone  BF  cone.  pat. 


104. 


7 % Immedial  Indone  BF  cone.  pat. 


105. 


3.5%  Immedial  Indone  4B  cone.  pat. 


106. 


% Immedial  Indone  4B  cone.  pat. 


107. 


3.5%  Immedial  Indone  3B  cone.  pat. 


108. 


7 % Immedial  Indone  3B  cone.  pat. 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


III 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


109. 

3.5%  Iiiimedial  Indone  EB  cone.  pat. 

110. 

7 % Immedial  Indone  RB  cone.  pat. 

111. 

4 % Immedial  Indone  EG  cone.  pat. 

112. 

8 % Immedial  Indone  EG  cone.  pat. 

113. 

3 % Immedial  Indone  RE  cone.  pat. 

114. 

6 % Immedial  Indone  RE  cone.  pat. 

115. 

3 % Immedial  Indone  R cone.  pat. 


127. 

3.5%  Immedial  Blue  CBL  extra  cone.  pat. 
Immedial  Developer. 

128. 

7 % Immedial  Blue  CBL  extra  cone.  pat. 
Immedial  Developer. 

129. 

3.5%  Immedial  Blue  CR  extra  cone.  pat. 
Immedial  Developer. 

130. 

7 % Immedial  Blue  CR  extra  cone.  pat. 
Immedial  Developer. 

131. 

3.5%  Immedial  Blue  CRBN  extra  cone.  pat. 
Immedial  Developer. 


116. 

C % Immedial  Indone  R cone.  pat. 

117. 

4 % Immedial  New  Blue  G cone.  pat. 
Immedial  Developer. 

118. 

8 % Immedial  New  Blue  G cone.  pat. 
Immedial  Developer. 


132. 

7 % Immedial  Blue  CRBN  extra  cone.  pat. 
Immedial  Developer. 

133. 

3.5%  Immedial  Direct  Blue  FCL  extra  cone. 

pat. 

134. 

7 % Immedial  Direct  Blue  FCL  extra  cone. 

. P^t. 


119. 

3 % Immedial  Indone  Violet  B cone.  pat. 

120. 

7 % Immedial  Indone  Violet  B cone.  pat. 

121. 

3.5%  Immedial  Blue  CB  extra  cone.  pat. 
J^mmedial  Developer. 

122. 

7 % Immedial  Bli’.e  CB  extra  cone.  pat. 
Immedial  Developer. 

123. 

3.5%  Immedial  Blue  CRB  e.xtra  cone.  pat. 
Immedial  Developer. 

124. 

7 % Immedial  Blue  CRB  extra  cone.  pat. 
Immedial  Devekper. 

125. 

3.5%  Immedial  Blue  C e.xtra  cone.  pat. 
Immedial  Developer. 

126. 

7 % Immedial  Blue  C extra  cone.  pat. 
Immedial  Developer. 


135. 

3.5%  Immedial  Direct  Blue  JND  extra  cone. 

pat. 

136. 

7 % Immedial  Direct  Blue  JND  extra  cone. 

pat. 

137. 

4 % Immedial  Dark  Blue  CRV  pat. 

138. 

8 % Immedial  Dark  Blue  CRV  pat. 

139 

4 %;  Immedial  Direct  Blue  4B  extra  cone.  pat. 

140. 

7 % Immedial  Direct  Blue  4B  extra  cone.  pat. 

141. 

3.5%  Immedial  Direct  Blue  RC  extra  cone.  pat. 

142. 

7 % Immedial  Direct  Blue  RC  extra  cone.  pat. 

143. 

3.5%  Immedial  Direct  Blue  B extra  cone.  pat. 

144. 

7 % Immedial  Direct  Blue  B extra  cone.  pat. 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IV 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


145. 

163. 

3.5  % Immedial  Dark  Blue  JB  pat. 

0.75%  Immedial  Carbon  B. 

146. 

164. 

7 % Immedial  Dark  Blue  JR  pat. 

5 % Immedial  Carbon  B. 

147. 

165. 

3.5  % Immedial  Direct  Blue  BB  extra  cone. 

pat. 

1.2  % Immedial  Brilliant  Black  5BV  cone. 

pat 

148. 

166. 

7 % Immedial  Direct  Blue  BB  extra  cone. 

pat. 

8 % Immedial  Brilliant  Black  5BV  cone. 

pat 

149. 

167. 

3.5  % Immedial  Dark  Blue  J pat. 

0.75%  Immedial  Brilliant  Carbon  F pat. 

150. 

7 % Immedial  Dark  Blue  J pat. 

168. 

5 % Immedial  Brilliant  Carbon  F pat. 

151. 

3.5  % Immedial  Direct  Blue  JB  extra  cone. 

pat. 

169. 

1.2  %^  Immedial  Black  NBB  cone. 

152. 

170. 

7 % Immedial  Direct  Blue  JB  extra  cone. 

pat. 

8 % Immedial  Black  NBB  cone. 

153. 

171. 

0.75%  Immedial  Carbon  BL. 

1.2  % Immedial  Black  BF  cone. 

154. 

172. 

5 % Immedial  Carbon  BL. 

8 % Immedial  Black  BF  cone. 

155. 

173. 

0.75%  Immedial  Carbon  R. 

1.2  % Immedial  Black  NNZ  cone. 

156. 

174. 

5 % Immedial  Carbon  R. 

8 % Immedial  Black  NNZ  cone. 

157. 

175. 

1.2  % Immedial  Brilliant  Black  BB  cone.  pat. 

1.2  % Immedial  Black  NNG  cone. 

158. 

176. 

8 % Immedial  Brilliant  Black  BB  cone.  pat. 

8 % Immedial  Black  NNG  cone. 

159. 

177. 

0.75%  Immedial  Carbon  JHJ. 

1.2  % Immedial  Black  NN  cone. 

160. 

178. 

5 % Immedial  Carbon  JIIJ. 

8 % Immedial  Black  NN  cone. 

161. 

179. 

0.75%  Immedial  Brilliant  Carbon  FG  pat. 

1.2  % Immedial  Black  NLN  cone. 

162. 

180. 

5 % Immedial  Brilliant  Carbon  FG  pat. 

8 % Immedial  Black  NLN  cone. 

IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


145  146  147  148 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


V 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


I 


181. 

0.6  % Immedial  Deep  Green  G pat. 

0.8  % Immedial  Direct  Blue  B pat. 

182. 

0.6  % Immedial  Direct  Blue  B pat. 

1.11  % Immedial  Deep  Green  G pat. 

0.3  % Immedial  Yellow  Olive  G pat. 

183. 

1.7  % Immedial  Direct  Blue  B pat. 

0.7  % Immedial  Dark  Brown  D cone.  pat. 

184. 

1 % Immedial  Black  NNG  cone. 

0.8  % Immedial  Brown  BR. 

185. 

0.08%  Immedial  Carbon  B 

0.08%  Immedial  Dark  Brown  D cone.  pat. 

186. 

0.23%  Immedial  Black  NNG  cone. 

0.08%  Immedial  Dark  Brown  D cone.  pat. 

187. 

0.4  % Immedial  Direct  Blue  B pat. 

0.3  % Immedial  Dark  Brown  D cone.  pat. 

188. 

1 % Immedial  Direct  Blue  B pat. 

0.35%  Immedial  Prime  S pat. 

0.4  % Immedial  Dark  Brown  D cone.  pat. 

189. 

1 % Immedial  Direct  Blue  B pat. 

1.5  % Immedial  Dark  Green  B 
0.6  % Immedial  Black  NNG  cone. 

190. 

0.75%  Immedial  Black  NNG  cone. 

0.75%  Immedial  Dark  Brown  D cone.  pat. 

191. 

0.4  % Immedial  Direct  Blue  B pat. 

0.12%  Immedial  Yellow  Olive  5G  pat. 

0.4  % Immedial  Dark  Brown  D cone.  pat. 

192. 

0.7  % Immedial  Direct  Blue  B pat. 

0.05%  Immedial  Carbon  B 

0.6  % Immedial  Dark  Brown  D cone.  pat. 

193. 

1 % Immedial  Direct  Blue  B pat. 

1.3  % Immedial  Dark  Green  B 
0.4  % Immedial  Black  NNG  cone. 

194. 

3 % Immedial  Direct  Blue  B pat. 

1 % Immedial  Yellow  Olive  G pat. 

195. 

0.65%  Immedial  Direct  Blue  B pat. 

0.8  % Immedial  Dark  Brown  D cone.  pat. 

196. 

1 % Immedial  Direct  Blue  B pat. 

0.6  % Immedial  Carbon  B 

0.8  % Immedial  Dark  Brown  D cone.  pat. 

197. 

1.5  % Immedial  Carbon  B 

0.8  % Immedial  Direct  Blue  B pat. 

0.35%  Immedial  Dark  Brown  D cone.  pat. 

198. 

1.4  % Immedial  Carbon  B 

0.3  % Immedial  Dark  Brown  D cone.  pat. 
0.6  % Immedial  Prune  S pat. 


199. 

2.5  % Immedial  Dark  Green  B 

3 % Immedial  Direct  Blue  B pat. 

200. 

1.5  % Immedial  Black  NNG  cone. 

1 % Immedial  Direct  Blue  B pat. 

0.6  % Immedial  Prune  S pat. 

201. 

0.3  % Immedial  Direct  Blue  B pat. 

0.15%  Immedial  Prune  S pat. 

0.15%  Immedial  Carbon  KBL. 

202. 

1.5  % Immedial  Direct  Blue  B pat. 

1.2  % Immedial  Dark  Green  B 

203. 

2.5  % Immedial  Direct  Blue  B pat. 

1 % Immedial  Yellow  Olive  G pat. 

204. 

1.2  % Immedial  Dark  Green  B 

2.5  % Immedial  Direct  Blue  B pat. 

205. 

0.45%  Immedial  Direct  Blue  B pat. 

0.1  % Immedial  Yellow  Olive  5G  pat. 

0.6  % Immedial  Dark  Brown  D cone.  pat. 

206. 

0.6  % Immedial  Carbon  B 

0.3  % Immedial  Yellow  Olive  5G  pat. 

207. 

2 % Immedial  Direct  Blue  B pat. 

1 % Immedial  Dark  Green  B 

208. 

1.75%  Immedial  Carbon  B 
0.5  % Immedial  Prune  S pat. 

0.9  % Immedial  Direct  Blue  B pat. 

209. 

0.3  % Immedial  Cutcb  BGG  pat. 

0.55%  Immedial  Yellow  Olive  G pat. 

210. 

1.4  % Immedial  Cutcb  BGG  pat. 

0.4  % Immedial  Deep  Green  G pat. 

0.2  % Immedial  Brown  W cone.  pat. 

211. 

1.5  % Immedial  Cutcb  BGG  pat. 

0.4  % Immedial  Deep  Green  G pat. 

0.3  % Immedial  Brown  W cone.  pat. 

212. 

1.5  % Immedial  Cutcb  BGG  pat. 

0.5  % Immedial  Dark  Brown  D cone.  pat. 

213. 

1.4  % Immedial  Cutcb  BGG  pat. 

0.7  % Immedial  Yellow  Olive  5G  pat. 

0.3  % Immedial  Dark  Brown  D cone.  pat. 

214. 

3 % Immedial  Brown  BR 

1.3  % Immedial  Yellow  Olive  5G  pat. 

215. 

1.7  Immedial  Brown  BR 

0.5  % Immedial  Yellow  Olive  5G  pat. 

1 % Immedial  Dark  Brown  D cone.  pat. 

216. 

4.5  % Immedial  Cutcb  BGG  pat. 

1.3  % Immedial  Yellow  Olive  5G  pat. 


VI 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


2 % 

0.7  % 


1.7  % 

1.8  % 


2.5  \ 
0.5  % 


6 % 
3 % 


4.5  % 
2 % 


2.6  o/o 

1 % 


5.5  % 

1.5  % 


1.2  % 
0.6  % 
0.2  % 


1.25% 

0.8  % 


/O 

2.2  % 


1 % 

4.5  % 


2.5  % 
2.5  % 


2 % 

3.8  % 


2 % 
1 % 
0.5  % 


1.5  % 
1 To 
0.3  % 


1 % 
0.8  % 


0.2  % 
0.25% 
0.25% 


0.8  % 
0.6  % 


217. 

Immedial  Yellow  Olive  5G  pat. 
Immedial  Yellow  D pat. 

218. 

Immedial  Yellow  GG  pat. 

Immedial  Yellow  Olive  5G  pat. 

219. 

Immedial  Yellow  Olive  5G  pat. 
Immedial  Yellow  D pat. 

220. 

Immedial  Yellow  D pat. 

Immedial  Yellow  Olive  G pat. 

221. 

Immedial  Cutch  BGG  pat. 

Immedial  Dark  Brown  D cone.  pat. 

222. 

Immedial  Bordeaux  GF  cone.  pat. 
Immedial  Cutch  0 pat. 

223. 

Immedial  Yellow  D pat. 

Immedial  Orange  C pat. 

224. 

Immedial  Cutch  BGG  pat. 
Immedial  Yellow  Olive  5G  pat. 
Immedial  Dark  Brown  D cone.  pat. 

225. 

Immedial  Yellow  Olive  5G  pat. 
Immedial  Cutch  0 pat. 

226. 

Immedial  Cutch  0 pat. 

Immedial  Yellow  Olive  G pat. 

227. 

Immedial  Yellow  Olive  G pat. 
Immedial  Cutch  BGG  pat. 

228. 

Immedial  Brown  BR 
Immedial  Cutch  0 pat. 

229. 

Immedial  Dark  Brown  D cone.  pat. 
Immedial  Yellow  Olive  G pat. 

230. 

Immedial  Cutch  BGG  pat. 

Immedial  Yellow  Olive  G pat. 
Immedial  Black  NNG  cone. 

231. 

Immedial  Cutch  BGG  pat. 
Immeilial  Yellow  Olive  5G  pat. 
Immedial  Dark  Brown  D cone.  pat. 

232. 

Immedial  Cutch  BGG  pat. 

Immedial  Dark  Brown  D cone.  pat. 

233. 

Immedial  Cutch  BGG  pat. 

Immedial  Black  NNG  cone. 
Immedial  Yellow  Olive  5G  pat. 

234. 

Immedial  Cutch  BGG  pat. 

Immedial  Dark  Green  B. 


235. 

0.3  % Immedial  Carbon  B 

1.5  % Immedial  Yellow  Olive  5G  pat. 
0.6  % Immedial  Brown  BR  pat. 

236. 

0.7  % Immedial  Dark  Brown  D cone. 

1.2  % Immedial  Yellow  Olive  G pat. 

237. 

0.65%  Immedial  Cutch  BGG  pat. 

238. 

0.8  % Immedial  Cutch  BGG  pat. 

0.1  % Immedial  Yellow  Olive  G pat. 
0.05%  Immedial  Black  NNG  cone. 

239. 

1 % Immedial  Cutch  BGG  pat. 

0.8  % Immedial  Yellow  Olive  5G  pat. 
0.4  % Immedial  Dark  Brown  D cone.  i 

240. 

1 % Immedial  Cutch  BGG  pat. 

0.15%  Immedial  Yellow  Olive  G pat. 
0.25%  Immedial  Black  NNG  cone. 

241. 

2.2  % Immedial  Cutch  BGG  pat. 

0.3  % Immedial  Yellow  Olive  G pat. 

242. 

2 % Immedial  Cutch  BGG  pat. 

0.06%  Immedial  Carbon  B. 

243. 

4.5  % Immedial  Cutch  BGG  pat. 

4.5  % Immedial  Yellow  Olive  5G  pat. 
0.6  % Immedial  Carbon  B. 

244. 

1.5  % Immedial  Green  Yellow  G pat. 

5.5  % Immedial  Cutch  BGG  pat. 

245. 

5 %/Immedial  Yellow  GG  pat. 

1.2  % Immedial  Orange  C pat. 

246. 

2 % Immedial  Cutch  0 pat. 

3.5  % Immedial  Yellow  D pat. 

247. 

3 % Immedial  Orange  C pat. 

4.5  % Immedial  Yellow  D pat. 

248. 

2.5  % Immedial  Cutch  0 pat. 

0.5  % Immedial  Maroon  B cone.  pat. 

249. 

2 % Immedial  Brown  BR 

1.5  % Immedial  Maroon  B cone.  pat. 

250. 

3 % Immedial  Bordeaux  GF  cone. 

0.7  % Immedial  Cutch  BGG  pat. 

251. 

2 % Immedial  Brown  BR. 

252. 

3 % Immedial  Bro\vn  BR 

1.2  % Immedial  Dark  Brown  D cone. 
0.5  % Immedial  Carbon  B. 


VII 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


253. 

1.2  % Immedial  Yellow  GG  pat. 

1.2  % Immedial  Yellow  Olive  5G  pat. 

0.065%  Immedial  Green  GGX  cone.  pat. 

254. 

1.5  % Immedial  Yellow  GG  pat. 

0.7  % Immedial  Yellow  Olive  5G  pat. 

0.3  % Immedial  Green  GGX  cone.  pat. 

255. 

2 % Immedial  Yellow  Olive  5G  pat. 

0.3  % Immedial  Black  NN(j  cone. 

256. 

4 % Immedial  Yellow  Olive  5G  pat. 

0.8  % Immedial  Deep  Green  G pat. 

257. 

6 % Immedial  Yellow  Olive  5G  pat. 

1.2  % Immedial  Deep  Green  G pat. 

258. 

1.7  % Immedial  Yellow  Olive  5G  pat. 

0.3  % Immedial  Black  NNG  cone. 

259. 

9 % Immedial  Yellow  Olive  5G  pat. 

0.7  % Immedial  Carbon  B 

0.7  % Immedial  Dark  Brown  D cone.  pat. 

260. 

1.5  % Immedial  Yellow  Olive  5G  pat. 

0.3  % Immedial  Carbon  B 

0.7  % Immedial  Dark  Brown  D cone.  pat. 

261. 

2.3  % Immedial  Green  Yellow  G pat. 

2 % Immedial  Dark  Green  B 

1 % Immedial  Cutch  O pat. 

262. 

5 % Immedial  Green  Yellow  G pat. 

3.4  % Immedial  Dark  Green  B 

2.8  % Immedial  Cutch  0 pat. 

263. 

2 % Immedial  Green  Yellow  G pat. 

1.5  % Immedial  Dark  Green  B 

3 % Immedial  Cutch  0 pat. 

264. 

2.5  % Immedial  Green  Yellow  G pat. 

1.5  % Immedial  Dark  Green  B 

2.5  % Immedial  Cutch  0 pat. 

265. 

3.25  % Immedial  Green  Yellow  G pat. 

2 % Immedial  Dark  Green  B 

5 % Immedial  Cutch  0 pat. 

266. 

2.8  % Immedial  Green  Yellow  G pat. 

2 % Immedial  Dark  Green  B 

4.7  % Immedial  Cutch  O pat. 

267. 

4 % Immedial  Green  Yellow  G pat. 

2.8  % Immedial  Dark  Green  B 

2.3  % Immedial  Cutch  O pat. 

268. 

4.7  % Immedial  Green  Yellow  G pat. 

4.7  % Immedial  Dark  Green  B. 


269. 

4.7  % Immedial  Green  Yellow  G pat. 

2 % Immedial  Dark  Green  B. 

270. 

8 % Immedial  Green  Yellow  G pat. 

2.8  % Immedial  Dark  Green  B. 

271. 

5.4  % Immedial  Green  Yellow  G pat. 

5.4  % Immedial  Dark  Green  B. 

272. 

3 % Immedial  Green  Yellow  G pat. 

3 % Immedial  Dark  Green  B. 

273. 

3.5  % Immedial  Yellow  Olive  G pat. 

0.9  % Immedial  Carbon  B 

0.2  % Immedial  Dark  Brown  D cone.  pat. 

274. 

1.3  % Immedial  Yellow  Olive  G pat. 

0.4  % Immedial  Carbon  B 

1.2  % Immedial  Dark  Brown  D cone.  pat. 

275. 

1.5  % Immedial  Yellow  Olive  5G  pat. 

0.5  % Immedial  Black  NNG  cone. 

0.1  % Immedial  Deep  Green  G pat. 

276. 

1 % Immedial  Dark  Brown  D cone.  pat. 

1.2  % Immedial  Olive  B pat. 

277. 

8 % Immedial  Deep  Green  G pat. 

0.7  % Immedial  Carbon  B. 

278. 

4.5  % Immedial  Deep  Green  G pat. 

0.9  % Immedial  Dark  Green  B 

1.9  % Immedial  Yellow  Olive  5G  pat. 

279. 

0.7  % Immedial  Carbon  B 
5 % Immedial  Green  Blue  CV  pat. 

3.5  % Immedial  Yellow  Olive  G pat. 

280. 

1.4  % Immedial  Carbon  B 

3.5  % Immedial  Green  Blue  CV  pat. 

3.5  % Immedial  Yellow  Olive  G pat. 

281. 

3 % Immedial  Yellow  Olive  5G  pat. 

1.6  % Immedial  Carbon  B 

282. 

1.5  % Immedial  Carbon  B 

4 % Immedial  Yellow  Olive  G pat. 

283. 

0.7  % Immedial  Carbon  B 

2.5  % Immedial  Yellow'  Olive  G pat. 

0.4  % Immedial  Dark  Brown  D cone.  pat. 

284. 

2.5  % Immedial  Dark  Green  B 
0.5  % Immedial  Carbon  B. 

285. 

3 % Immedial  Dark  Green  B 

0.5  % Immedial  Yellow'  Olive  G pat. 

286. 

8 % Immedial  Dark  Green  B 

2.2  % Immedial  Cutch  O pat. 

2 % Immedial  Green  GG  extra  pat. 

287. 

2 % Immedial  Olive  B pat. 

0.5  % Immedial  Dark  Brown  D cone.  pat. 

288. 

1.5  % Immedial  Direct  Blue  B pat. 

2 % Immedial  Yellow  Olive  G pat. 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


VIII 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


0.6  % 
0.2  % 

0.5  % 
0.05% 

1.8  % 
0.2  % 

1.5  % 
1.8  % 
0.3  % 

2 % 

0.15% 

0.05% 

1.8  % 
0.4  % 

0.15% 

3.6  % 
0.4  % 

0.1  % 
5 % 

0.3  % 

2.5  % 
0.7  % 

2.5  % 

0.15% 
0.2  % 

3.6  % 
0.5  % 

7 % 

1.8  % 

1.8  % 
2.2  % 
0.6  % 

2.9  % 
1-2  % 

5 % 

1-4  % 

2.8  % 
2.2  % 

3.8  % 
0.3  % 

2.5  % 
2.5  % 


289 

Immedial  Green  GG  extra  pat. 
Immedial  Yellow  Olive  G pat. 

290. 

Immedial  Green  BB  extra  pat. 
Immedial  Yellow  Olive  5G  pat. 

291. 

Immedial  Green  BB  extra  pat. 
Immedial  Carbon  B. 

292. 

Immedial  Green  BB  extra  pat. 
Immedial  Indogene  GCL  cone.  pat. 
Immedial  Yellow  Olive  5G  pat. 

293. 

Immedial  Green  BB  extra  pat. 

topped  with 

Brilliant  Green  Crystals  extra 
Methylene  Blue  BB. 

294. 

Immedial  Deep  Green  G pat. 
Immedial  Yellow  Olive  5G  pat. 
topped  with 

Brilliant  Green  Crystals  extra 

295. 

Immedial  Deep  Green  G pat. 
Immedial  \ellow  Olive  5G  pat. 

topped  with 

Brilliant  Green  Crystals  extra 

296. 

Immedial  Green  BB  extra  pat. 
Immedial  Indogene  GCL  cone.  pat. 

297. 

Immedial  Green  GG  extra  pat. 
Immedial  Green  Blue  CV  pat. 

298. 

Immedial  Brilliant  Green  G extra  pat. 

topped  with 

Brilliant  Green  Crystals  extra 
Thioflavine  TCN. 


Immedial 

Immedial 

Immedial 

Immedial 

Immedial 

Immedial 

Immedial 


Immedial 

Immedial 


Immedial 

Immedial 

Immedial 

Immedial 

Immedial 

Immedial 

Immedial 

Immedial 


299. 

Green  GG  extra  pat. 
Green  Blue  CV  pat. 

300. 

Green  GGX  cone.  pat. 
Y'ellow  D pat. 

301. 

Yellow  GG  pat. 
Yellow  Olive  5G  pat. 
Green  GG  extra  pat. 

302. 

Yellow  Olive  5G  pat. 
Deep  Green  G pat. 

303. 

Yellow  GG  pat. 

Green  GG  extra  pat. 

304. 

Yellow  Olive  5G  pat. 
Green  GG  extra  pat. 

305. 

Green  GG  extra  pat. 
Yellow  Olive  5G  pat. 

306. 

Green  Blue  CV  pat. 
Yellow  Olive  5G  pat. 


307. 

1.6  % Immedial  Green  GG  extra  pat, 

1 % Immedial  Yellow  Olive  G pat. 

308. 

8 % Immedial  Green  GG  extra  pat. 

2.8  % Immedial  Yellow  GG  pat. 

309. 

3 % Immedial  Green  GG  extra  pat. 

2.5  % Immedial  Y'ellow  GG  pat. 

310. 

0.7  % Immedial  Dark  Green  B 
2.2  % Immedial  Green  GG  extra  pat. 

2.5  % Immedial  Yellow  Olive  5G  pat. 

311. 

1 % Immedial  Yellow  D pat. 

3.5  % Immedial  Green  GG  extra  pat. 

312. 

5 % Immedial  Green  GG  extra  pat. 

0.7  % Immedial  Yellow  Olive  G pat. 

313. 

8 % Immedial  Green  GG  extra  pat. 

2 % Immedial  Y’ellow  GG  pat. 

314. 

1 % Immedial  Dark  Green  B pat. 

2 % Immedial  Deep  Green  G pat. 

1 % Immedial  Yellow  Olive  G pat. 

315. 

4 % Immedial  Deep  Green  G pat. 

5 % Immedial  Yellow  Olive  G pat. 

316. 

8 % Immedial  Deep  Green  G pat. 

0.9  % Immedial  Yellow  Olive  5G  pat. 

0.3  % Immedial  Carbon  B. 

317. 

1.5  % Immedial  Yellow  Olive  5G  pat. 

2.2  % Immedial  Dark  Green  B. 

318. 

3.8  % Immedial  Yellow  Olive  5G  pat. 

0.5  % Immedial  Carbon  B. 

319. 

8 % Immedial  Yellow  Olive  5G  pat. 

1.5  % Immedial  Carbon  B. 

320. 

4.5  % Immedial  Deep  Green  G pat. 

0.7  % Immedial  Yellow  Olive  G pat. 

0.5  % Immedial  Carbon  B. 

321. 

6 % Immedial  Cutch  OG  pat. 

4.5  % Immedial  Dark  Brown  D cone.  pat. 

1.5  % Immedial  Carbon  B. 

322. 

4 % Immedial  Dark  Brown  D cone.  pat. 

4.5  % Immedial  Yellow  Olive  5G  pat. 

2.5  % Immedial  Dark  Green  B. 

323. 

4.5  % Immedial  Cutch  OG  pat. 

4.5  % Immedial  Dark  Brown  D cone.  pat. 

2 % Immedial  Carbon  B. 

324. 

7.5  % Immedial  Dark  Brown  D cone.  pat. 

3.5  % Immedial  Yellow  Olive  5G  pat. 

4 % Immedial  Dark  Green  B. 


IMMEDIAL  COLOUKS  ON  LOOSE  COTTON 


CASSELLA  COLOK  COMPANY,  NEW  YORK. 


IX 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


325. 

0.3  % Immedial  Green  GG  extra  pat. 

0.1  % Immedial  Indogene  GCL  cone.  pat. 

326. 

0.1  % Immedial  Green  GG  extra  pat. 

0.4  % Immedial  Indogene  GCL  cone.  pat. 

327. 

0,2  % Immedial  Green  GG  extra  pat. 

0.2  % Immedial  Indogene  GCL  cone.  pat. 

328. 

0.8  % Immedial  Green  BB  extra  pat. 

0.7  % Immedial  Indogene  GCL  cone.  pat. 

329. 

0.8  % Immedial  Indogene  GCL  cone.  pat. 
0.4  % Immedial  Green  Blue  CV  pat. 

330. 

1 % Immedial  Indogene  GCL  cone.  pat. 

0.35%  Immedial  Green  BB  extra  pat. 

331. 

1 % Immedial  Indogene  GCL  cone.  pat. 

1 % Immedial  Indogene  BCL  cone.  pat. 

topped  with 

0.05%  Methylene  Blue  BB. 

332. 

1.8  % Immedial  Indogene  GCL  cone.  pat. 
0.3  % Immedial  Green  GG  extra  pat. 

333. 

0.7  % Immedial  Green  GG  extra  pat. 

2 % Immedial  Indogene  GCL  cone.  pat. 

334. 

5 % Immedial'Indogene  GCL  cone.  pat. 

2.5  % Immedial  Green  BB  extra  pat. 

335. 

0.3  % Immedial  Green  GG  extra  pat. 

1.8  % Immedial  Indogene  GCL  cone.  pat. 


343. 

3.5  % Immedial  Indogene  GCL  cone.  pat. 
0.75%  Immedial  Deep  Green  G pat. 

344. 

2 % Immedial  Deep  Green  G pat. 

2.5  % Immedial  Direct  Blue  B pat. 

345. 

6 % Immedial  Deep  Green  G pat. 

0.7  % Immedial  Yellow  Olive  G pat. 

1.5  % Immedial  Carbon  B. 

346. 

7 % Immedial  Deep  Green  G pat. 

3 % Immedial  Direct  Blue  B pat. 

347. 

7.5  % Immedial  Green  GG  extra  pat. 

2.2  % Immedial  Black  NNG  cone. 

348. 

2.2  % Immedial  Direct  Blue  4B  extra  pat. 

1.8  % Immedial  Deep  Green  G pat. 

349. 

0.75%  Immedial  Direct  Blue  B pat. 

350. 

1 % Immedial  Deep  Green  G pat. 

2.5  % Immedial  Direct  Blue  B pat. 

351. 

1.8  % Immedial  Direct  Blue  B pat. 

1.5  % Immedial  Green  BB  extra  pat. 

352. 

2 % Immedial  Direct  Blue  B pat. 

0.25%  Immedial  Green  BB  extra  pat. 

353. 

0.9  % Immedial  Direct  Blue  BB  extra  cone. 
1 % Immedial  Green  GG  extra  pat. 


336. 

3.5  % Immedial  Indogene  GCL  cone.  pat. 
0.25%  Immedial  Direct  Blue  B pat. 

337. 

1.8  % Immedial  Green  BB  extra  pat. 

1.8  % Immedial  Indogene  GCL  cone.  pat. 

338. 

3 % Immedial  Indone  3B  cone.  pat. 

1 % Immedial  Brilliant  Green  G extra 


3 % Immedial  Deep  Green  G pat. 

3 % Immedial  Indone  BBF  cone. 

340. 

2.6  % Immedial  Green  BB  extra  pat. 

2.2  % Immedial  Indogene  GCL  cone.  pat. 

341. 

2.2  % Immedial  Green  BB  extra  pat. 

0.8  % Immedial  Indogene  GCL  cone.  pat. 
0.2  % Immedial  Carbon  B. 

342. 

2.8  % Immedial  Green  BB  extra  pat. 

1.5  % Immedial  Indogene  GCL  cone.  pat. 
0.3  % Immedial  Carbon  B. 


354. 

1.5  % Immedial  Direct  Blue  BB  extra  cone. 
0.4  % Immedial  Green  BB  extra  pat. 

355. 

2.8  % Immedial  Direct  Blue  B pat. 

2.8  % Immedial  Green  Blue  CV  pat. 

356. 

3 % Immedial  Direct  Blue  B pat. 

3 % Immedial  Green  Blue  CV  pat. 

1.8  % Immedial  Indone  3B  cone.  pat. 

357. 

2 % Immedial  Indone  JBF  cone.  pat. 

0.5  % Immedial  Direct  Blue  BB  extra  cone. 

358. 

2.3  % Immedial  Direct  Blue  B pat. 

1.7  % Immedial  Indone  R cone.  pat. 

359. 

8 % Immedial  Indone  JBN  cone.  pat. 

0.5  % Immedial  Deep  Green  G pat. 

360. 

9 % Immedial  Indone  JBN  cone.  pat. 

0.5  % Immedial  Direct  Blue  B pat. 


X 


IMMEDIAL  COLOURS  ON  LOOSE  COTTON 


361. 

2 % Immedial  Indone  Violet  B cone.  pat. 

363. 

2 % Immedial  Indone  BBF  cone.  pat. 

topped  with: 

0.5  % New  Methylene  Blue  3E. 

363. 

4 % Immedial  Indone  R cone.  pat. 

3 % Immedial  Indone  Violet  B cone.  pat. 

364. 

2.8  % Immedial  Direct  Blue  B pat. 

2.5  % Immedial  Indone  R cone.  pat. 

366. 

1 % Immedial  Indogene  GCL  cone.  pat. 

4 % Immedial  Direct  Blue  B pat. 

366. 

5 % Immedial  Direct  Blue  R pat. 

1.8  % Immedial  Indone  RR  cone.  pat. 

1 % Immedial  Violet  CB. 

367. 

8 % Immedial  Indone  Violet  B cone.  pat. 

2 % Immedial  Direct  Blue  R pat. 

368. 

3 % Immedial  Direct  Blue  11  pat. 

3 % Immedial  Indone  RR  cone.  pat. 

369. 

2.5  % Immedial  Indone  Violet  B cone.  pat. 

2 % Immedial  Direct  Blue  B pat. 

370. 

3.5  % Immedial  Indone  Violet  B cone.  pat. 
0.25%  Immedial  Indone  R cone.  pat. 

371. 

7 % Immedial  Indone  Violet  B cone.  pat. 
0.7  % Immedial  Direct  Blue  B pat. 

372. 

8 % Immedial  Direct  Blue  B pat. 

373. 

0.2  % Immedial  Carbon  B 

0.7  % Immedial  Yellow  Olive  G pat. 

2  % Immedial  Dark  Brown  D cone.  pat. 

374. 

2 % Immedial  Dark  Brown  D cone.  pat. 

0.25%  Immedial  Black  NNG  cone. 

375. 

0.8  % Immedial  Dark  Brown  D cone.  pat. 
0.1  % Immedial  Yellow  Olive  G pat. 

0.2  % Immedial  Dark  Green  B. 

376. 

8 % Immedial  Yellow  Olive  5G  pat. 

0.8  % Immedial  Carbon  B 

0.8  % Immedial  Dark  Brown  D cone.  pat. 

377. 

6 % Immedial  Olive  B pat. 

2 % Immedial  Cutch  O pat. 

378. 

0.8  % Immedial  Carbon  B 

4.5  % Immedial  Yellow  Olive  G pat. 


379. 

6 % Immedial  Olive  B pat. 

1.5  % Immedial  Cutch  0 pat. 

380. 

4 % Immedial  Deep  Green  G pat. 

2 % Immedial  Cutch  0 pat. 

1.9  % Immedial  Yellow  Olive  5G  pat. 

381. 

4 % Immedial  Cutch  OR  pat. 

6 % Immedial  Brown  W cone.  pat. 

382. 

8 % Immedial  Cutch  OR  pat. 

1.8  % Immedial  Carbon  B. 

383. 

5.5  % Immedial  Cutch  OR  pat. 

5.5  % Immedial  Brown  W cone.  pat. 

384. 

8 % Immedial  Cutch  OR  pat. 

3 % Immedial  Brown  W cone.  pat. 

385. 

8 % Immedial  Dark  Brown  D cone.  pat. 

4 % Immedial  Yellow  Olive  5G  pat. 

1.8  % Immedial  Carbon  B. 

386. 

4 % Immedial  Dark  Brown  D cone.  pat. 

5.5  % Immedial  Yellow  Olive  5G  pat. 

1 % Immedial  Carbon  B. 

387 

3.5  % Immedial  Dork  Brown  D cone.  pat. 

6 % Immedial  Yellow  Olive  5G  pat. 

0.7  % Immedial  Carbon  B. 

388. 

7 % Immedial  Cutch  OG  pat. 

4 % Immedial  Dark  Brown  D cone.  pat. 

0.7  % Immedial  Carbon  B. 

389. 

8 % Immedial  Prune  S pat. 

1.5  % Immedial  Direct  Blue  B pat. 

390. 

10  % Immedial  Brown  W cone.  pat. 

2.2  % Immedial  Black  NNG  cone. 

391. 

1.5  % Immedial  Cutch  BGG  pat. 

10  % Immedial  Dark  Brown  D cone.  pat. 

*392. 

3 % Immedial  Brown  W cone.  pat. 

3 % Immedial  Dark  Brown  D cone.  pat. 

1.8  % Iirimedial  Brown  BR. 

393. 

6 % Immedial  Direct  Blue  B extra  cone. 

3 % Immedial  Carbon  B. 

394. 

4.5  % Immedial  Direct  Blue  B extra  cone. 

4 % Immedial  Carbon  B. 

395. 

2.5  % Immedial  Direct  Blue  B extra  cone. 

1.5  % Immedial  Carbon  B. 

396.  ' 

5 % Immedial  Direct  Blue  B extra  cone. 

1 % Immedial  Black  NNG  cone. 


IMxMEDIAL  COLOURS  ON  LOOSE  COTTON 


XI 


f- 


• -r 


n 


*>7A  ‘ 


■1--  ,(■ 

^ ‘I 


7 


. ■■  ■ -m 


•l^'  ' ^ fiBUl  ’’ 

..r  ^-'M. 


%T 


'■V:’ 


■'VI  ■ ' . 


:ii! 


7 -^,’^’  '7:' 

J '•  f ’ s/ 


, ^ 

( 


» 


■il: 


I » 


( 

'r 


r' 

\ 


'■V 


■' 

j.-\, 
‘A’.  ' 


(t  • 


V ^ ' r : \jr^ 


^ ' 1_V 


-1 


•C 

#* 


w 


r;. 


/ 


r> 


- 7\ 


? 


' . .'^*5 


lUSSIAN  ANIMNK  COLOUR  WORKS  LEOPOLD  CASSELLA  & Co.,  RIGA. 


SfQ-C'O-^ 


G£n.  LLi 

LIBRARY 


Works  at  Riga. 


